A3V5O14 (A = K+, Rb+, or Tl+), New Polar Oxides with a Tetragonal Tungsten Bronze Related Structural Topology: Synthesis, Structure, and Functional Properties
Jeongho Yeon; Sang-Hwan Kim; P. Shiv Halasyamani; Inorganic Chemistry 49 (2010) 6986–6993; doi:10.1021/ic1008297

data_4316138
_publ_contact_author_address
;
Department of Chemistry
University of Houston
Houston, Texas
77204-5003
USA
;
_publ_contact_author_email       psh@uh.edu
_publ_contact_author_fax         1-713-743-0796
_publ_contact_author_name        'P. Shiv Halasyamani'
_publ_contact_author_phone       1-713-743-3278
_publ_section_title
;
 A3V5O14 (A = K+, Rb+, or Tl+), New Polar Oxides with a Tetragonal
 Tungsten Bronze Related Structural Topology: Synthesis, Structure, and
 Functional Properties
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6986
_journal_page_last               6993
_journal_paper_doi               10.1021/ic1008297
_journal_volume                  49
_journal_year                    2010
_chemical_absolute_configuration unk
_chemical_formula_sum            'O14 Tl3 V5'
_chemical_formula_weight         1091.81
_chemical_name_systematic
;

 ?

;
_space_group_IT_number           157
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'P 3 -2'
_symmetry_space_group_name_H-M   'P 3 1 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   8.7397(8)
_cell_length_b                   8.7397(8)
_cell_length_c                   5.0846(10)
_cell_measurement_temperature    296(2)
_cell_volume                     336.34(8)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 0.976
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0267
_diffrn_reflns_av_unetI/netI     0.0252
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            2117
_diffrn_reflns_theta_full        25
_diffrn_reflns_theta_max         28.72
_diffrn_reflns_theta_min         2.69
_exptl_absorpt_coefficient_mu    39.173
_exptl_absorpt_correction_T_max  0.6954
_exptl_absorpt_correction_T_min  0.6954
_exptl_absorpt_correction_type   psi-scan
_exptl_crystal_density_diffrn    5.39
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             470
_exptl_crystal_size_max          0.01
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         0.849
_refine_diff_density_min         -0.758
_refine_diff_density_rms         0.15
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.004(8)
_refine_ls_extinction_coef       0.0092(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.096
_refine_ls_matrix_type           full
_refine_ls_number_parameters     41
_refine_ls_number_reflns         592
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.095
_refine_ls_R_factor_all          0.0159
_refine_ls_R_factor_gt           0.0156
_refine_ls_shift/su_max          0.006
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0124P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0309
_refine_ls_wR_factor_ref         0.031
_reflns_number_gt                582
_reflns_number_total             592
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic1008297_si_002_3.cif
_cod_data_source_block           Tl3V5O14
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Trigonal' changed to 'trigonal'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Psi scan'
changed to 'psi-scan' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4316138